Scratching as a fracture process: from butter to steel The MIT Faculty has made this article openly available. Please share how this access benefits you. Your story matters. Citation Akono, A-T., P. Reis, and F-J. Ulm. “Scratching as a Fracture Process: From Butter to Steel.” Physical Review Letters 106.20 (2011): 204302.© 2011 American Physical Society. As Published http://dx.doi.org/10.1103/PhysRevLett.106.204302 Publisher American Physical Society Version Final published version Accessed Thu May 26 19:27:02 EDT 2016 Citable Link http://hdl.handle.net/1721.1/65375 Terms of Use Article is made available in accordance with the publisher's policy and may be subject to US copyright law. Please refer to the publisher's site for terms of use. Detailed Terms PRL 106, 204302 (2011) week ending 20 MAY 2011 PHYSICAL REVIEW LETTERS Scratching as a Fracture Process: From Butter to Steel A-T. Akono,1 P. M. Reis,1,2 and F-J. Ulm1,* 1 Department of Civil and Environmental Engineering, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139, USA 2 Department of Mechanical Engineering, Massachusetts Institute of Technology, Cambridge 02139, USA (Received 8 December 2010; published 20 May 2011) We present results of a hybrid experimental and theoretical investigation of the fracture scaling in scratch tests and show that scratching is a fracture dominated process. Validated for paraffin wax, cement paste, Jurassic limestone and steel, we derive a model that provides a quantitative means to relate quantities measured in scratch tests to fracture properties of materials at multiple scales. The scalability of scratching for different probes and depths opens new venues towards miniaturization of our technique, to extract fracture properties of materials at even smaller length scales. DOI: 10.1103/PhysRevLett.106.204302 PACS numbers: 46.50.+a, 46.25.y, 46.35.+z, 62.20.D Scooping cold butter with a knife [Fig. 1(a)] is a familiar experience. As the knife advances along an initially flat surface, it plows and cuts as small chips emanate in the process, leaving behind a well-defined groove. We regard the scooping of butter as a scratch test, which is probably one of the oldest techniques in the characterization of mechanical material properties. For instance, in 1824, Mohs’ hardness scale was introduced as an empirical way to quantify the scratch resistance of minerals [1]. Despite the apparent simplicity of this procedure, a fundamental understanding of the underlying mechanism remains aloof. The challenge lies in the difficulty to predictively rationalize the mechanisms that drive the scratch resistance vis-à-vis the chipping of material [Fig. 1(b)], with the shape and size dependence on the mechanical properties of the material, scratch depth and geometry of the scratch device. Nonetheless, the scratch test remains popular today in many applications involving material characterization, including adhesion properties of coatings [2], damage and wear of metals and polymers [3], strength of rocks [4], and skin biomechanics [5]. Here, we focus on scratching as a fracture process and approach this problem through a combination of wellcontrolled experiments, scaling analysis, and theory. First, we perform precision tests on paraffin wax, which we regard as a model material. Dimensional analysis enables us to identify the mechanical ingredients involved. We then develop a theoretical framework based on an energetic approach to rationalize the process. Our predictive model is turned into an inverse application to determine the fracture toughness for a wide range of materials, cutter-blade geometries, and length scales. A representative photograph of our experimental setup is presented in Fig. 1(b) and the corresponding schematic diagram of the simplified scratch-cutting test geometry in Fig. 1(c1). We consider paraffin wax for its thermal stability, nearly linear elasticity, and brittle mechanical properties. The tensile strength and fracture toughness of paraffin wax were determined by independent standard tests, 0031-9007=11=106(20)=204302(4) namely, the strength by uniaxial tension tests on finite plates with a centered hole, 0 ¼ 2:03 0:25 MPa, and the fracture toughness by 3-point bending pﬃﬃﬃﬃ tests on notched specimen, Kc ¼ 0:146 0:01 MPa m. A paraffin block (dimensions 3:4 5:7 22 cm) was clamped at its lateral sides, set on a linear stage and moved at constant velocity against a vertical steel cutter blade at depth d (measured from the block’s top surface). This blade of rectangular cross section (6.35 mm thick and w wide) was held by a rigid frame that ensured a constant depth and a zero backrake angle during the test. The values of w and d were a) b) 1cm 1cm z x 103 c1) z d) x 2 1 10 c2) 1 Crack = 2.5mm = 5mm = 10mm = 15mm = 20mm = 25mm 1 10 1 10 2 10 FIG. 1 (color online). (a) Scooping of butter with a knife. (b) Chips formation during the scratch test on paraffin wax. (c1) Schematic diagram of the scratch tests. (c2) Contour surface used in the J integral. (d) Tangential force, FT , versus projected area of the blade wd. A total number of 55 tests was carried out on paraffin wax with six different scratch widths, 2:5 w 25 mm, that were operated at five different depths, 2:5 d 12:5 mm. 204302-1 Ó 2011 American Physical Society PRL 106, 204302 (2011) PHYSICAL REVIEW LETTERS varied such that their aspect ratio was in the range 0:2 w=d 10. For each test, the horizontal and vertical forces generated, FT and FV , respectively, were recorded using load cells. In Fig. 1(d) we plot the dependence of the average of FT as a function of the blade’s projected contact area wd. For low values, FT scales linearly with wd which is significant of a strength process, in which the stress is limited by a threshold value that is the strength of the material, which is proportional to the slope of the curve FT ðwdÞ. However, for higher values of wd, deviations from this linear scaling are attributable to the fracture nature of the problem. We start by rationalizing the problem through a dimensional analysis of the quantities involved. Neglecting rate and thermal effects, we find that, FT w E w pﬃﬃﬃ ¼ ; (1) ; ; ðKc =0 Þ2 0 d Kc w d where Kc is the fracture toughness, 0 the material strength and E the Young’s modulus. The quantity ðKc =0 Þ2 has dimensions of length, and is characteristic (within a multiplying factor) of the size of the fracture process zone (FPZ) [6]. In Fig. 2 we reanalyze the original data [Fig. 1(b)], after making use of Eq. (1) to scale the results, and present thepﬃﬃﬃdependence of the normalized scratch force, FT =ðKc w dÞ versus w=d. Remarkably, the results for all different scratch widths and depths collapse onto a characteristic curve which converges for, pﬃﬃﬃw=d > 2, to a horizontal asymptote of approximately 2. In this domain, the width-to-FPZ ratio is w=rp 1, where the characteristic FPZ size is determined to be rp ¼ ð=8ÞðKc =0 Þ2 ¼ 2:0 mm, which indicates the validity of applying linear elastic fracture mechanics (LEFM) to our problem. Stress concentration at the blade edges for low w=d may entail plastic dissipation, pﬃﬃﬃ which is why the experimental values converge to 2 for large width-todepth ratios reminiscent of a fracture process. 5 =2.5mm =5mm =10mm =15mm =20mm =25mm Theory 4 3 2 1 0 −1 10 0 10 1 10 FIG. 2. Fracture scaling of the scratch tests on paraffin wax for blades with 2:5 w 25 mm and 2:5 d 12:5 mm. Same rawpﬃﬃﬃdata as in Fig. 1(d). The solid horizontal line is located at 2. week ending 20 MAY 2011 We proceed by developing a quantitative theoretical framework that explains this fracture behavior. The aim is to thereby be able to determine the fracture toughness Kc from the measured tangential force, FT , the scratch width, w, and scratch depth, d. Consider a linear elastic fracture process, in the simplified geometry illustrated in Fig. 1(c1). The spontaneous change in potential energy of the system, Epot , is due to the creation of a new fracture surface ¼ p‘, where p is the perimeter edge of the cutter blade, defining the crack tip geometry, and ‘ is the crack length. The energy release rate, G, is the thermodynamic driving force of crack propagation, and can be found from the relation, @Epot _ dEpot ¼ ¼ G p‘:_ @ dt (2) For planar crack growth, and within the framework of LEFM, the energy release rate can be estimated using a contour integral procedure, known as the J integral [7,8]. The fundamental idea of this method is to estimate the change in potential energy during a fracture process from the perspective of an observer attached to a propagating crack tip. Under displacement control, this observer witnesses two sources in the change of potential energy: one due to the change in free energy density, c , in a material volume, V, enclosing the crack tip; the other due to the energy release that is convectively transported at a speed _ x past the (fixed) observer: V n ¼ ‘n Z @c Z dEpot _ x dA; ¼ dV c ‘n dt V @t A (3) where A is the closed boundary of V, n the outward unit normal to A, and nx ¼ n ex . Developing the volume integral into a surface integral [9] for a linear elastic material, for which c ¼ 12 ij ui;j (ij is the stress tensor and ui;j is the displacement gradient), and then comparing Eqs. (2) and (3), yields the energy release rate, 1Z @u (4) c nx ti i dA; G¼ p A @x where ti ¼ ij ni are surface tractions. Compared to the classical form of the J integral [8], in which the fracture perimeter coincides with the fracture width, dA ¼ pds, we choose to consider a difference between these lengths, in order to later extend the technique to other scratch geometries. We hypothesize the existence of crack planes surrounding the blade and choose a closed volume that includes [Fig. 1(c2)] (i) the blade-material interface, the stress-free surface at the top (nx ¼ 0; ti ¼ 0), (ii) the (stress-free) fracture surfaces in prolongation of the scratch probe surface (nx ¼ 0; ti ¼ 0), and (iii) closing material surfaces far removed from the surfaces ( c ¼ 0; ui;x ¼ 0). Physically, the energy release so defined is associated with the energy stored, prior to chipping, into a material domain in front of the scratch blade. 204302-2 PRL 106, 204302 (2011) week ending 20 MAY 2011 PHYSICAL REVIEW LETTERS For the case of a rectangular blade (nx ¼ 1) of width w, the generated fracture surface is ¼ ðw þ 2dÞ‘. Noting that ti ¼ ij ni ¼ xx ex , xx ¼ FT =ðwdÞ; c ¼ 1 2 2 xx "xx ¼ xx =ð2EÞ; ux;x ¼ xx =E (where ¼ 1 for unconfined and ¼ 1 2 for confined stress state applications) and dS ¼ wdz, we readily obtain, G ¼ FT2 =½2Ew2 dð1 þ 2d=wÞ. As the scratch probe advances, fracture surfaces are generated along the probe’s bottom and lateral surfaces. In the process, a fracture energy Gc is released, which can be related to the fracture toughness as Gc ¼ Kc2 =E, [10]. Expressed in terms of the dimensionless expression of Eq. (1), the fracture propagation criterion therefore reads as, pﬃﬃﬃ FT d 1=2 pﬃﬃﬃ ¼ 2 1 þ 2 : (5) w Kc w d For large enough w=d ratios, Eq. (5) quantitatively confirms the fracture scaling of Eq.p(1) ﬃﬃﬃ and accurately describes the asymptotic value of 2 in the experimental results plotted in Fig. 2, for the scratch tests with paraffin. This opens the path for using the fracture criterion of Eq. (5) in an inverse application to determine the fracture toughness, Kc , for large values of w=d. We now explore the generality of our scratch fracture model, by predicting the fracture toughness in different experimental assays for two additional blade geometries, at different length scales: (i) an inclined rectangular cutter blade and (ii) a conical scratch device. In the first case, an inclined blade (back-rake angle and out-of-plane width w) is held at a depth d by a vertical force FV [Fig. 3(a), inset]. In contrast to the previous straight blade, FV is applied through the inclined surface and needs to be considered in the calculation. The classical J integral (w ¼ p) evaluated in this configuration [11] 2 yields J ¼ Feq =ð2Ew2 dÞ and Feq ¼ ðFT2 þ 35 FV2 Þ1=2 . Noting that the projected perimeter of the fracture surface is now p ¼ w þ 2d, and correcting for w=p, i.e. G ¼ ðw=pÞJ, we obtain a fracture criterion analogous to Eq. (5), pﬃﬃﬃ Feq d 1=2 pﬃﬃﬃ ¼ 2 1 þ 2 ; (6) w Kc w d where the tangential force is replaced by a force, Feq , that accounts for both FT and FV and drives the fracture process over the inclined blade-material interface. In Fig. 3 we apply this new fracture criterion to the experimental test of two materials—a cement paste and a Jurassic limestone—using the inclined blade geometry (15 pback-rake angle). In Figs. 3(a) and 3(c) we plot Feq ﬃﬃﬃﬃﬃﬃ vs w 2d, over a scratch path of 3.5 cm. Two observations deserve particular attention. First, the straight-line fits pﬃﬃﬃﬃﬃﬃ confirm the linearity between Feq and w 2d for each scratch width series. Moreover, the slope, which is representative for large values of w=d of the fracture toughness, decreases with the increase of the scratch width. In the a) 200 b) 1.1 =10mm =5mm =2.5mm Predicted 1.0 150 0.9 0.8 100 0.7 0.6 50 0.5 =10mm =5mm =2.5mm 0 0 50 100 150 200 250 c) 0.4 0.3 0.7 90 5 10 50 =15mm =10mm =5mm =2.5mm Predicted 100 50 0.6 80 60 0 0 10 20 110 d) 0.5 40 =15mm =10mm =5mm =2.5mm 20 0 0 100 200 300 0.4 0.3 4 10 50 80 FIG. 3 (color online). Fracture scaling of the scratch tests for cement paste and Jurassic limestone. (a), (b) Cement Paste. (c), (d) Jurassic limestone. The back-rake angle in all tests was 15 —inset (a). Three test series for cement paste and four series for limestone were conducted with scratch width, w ¼ 2:5 mm, 5 mm, 10 mm and 15 mm, and with scratch depth d ¼ 0:1–0:6 mm, spanning almost 2 orders of magnitude of w=d, from 5 to 100. linear fit of the data, we admit an offset value [Fig. 3(c), inset], which can be attributed to the highly localized plastic deformation at the contact of the indenter with the material. In Figs. 3(b) pﬃﬃﬃﬃﬃand ﬃ 3(d) we explore the same results, in terms of Feq =ðw 2dÞ vs w=d. As in the previous case for pﬃﬃﬃﬃﬃﬃ paraffin, Feq =ðw 2dÞ converges with w=d to a constant value that is representative of the fracture toughness. The mean value for cement paste toughness of Kcp¼ ﬃﬃﬃﬃﬃﬃ0:66 pﬃﬃﬃﬃ 0:05 MPa m obtained from averaging Feq =w 2d values for w=d > 10 is indeed in excellent agreement with reported fracture toughness values obtained by notched three-pointpﬃﬃﬃﬃ bending tests for large specimen, Kc ¼ 0:67 MPa m [12], or by means of extrapolation techniques thatpavoid interference with specimen size, Kc ¼ ﬃﬃﬃﬃ 0:65 MPa m [13]. We have also successfully employed this technique for other geomaterials, including sandstone and cemented siltstone. Finally, we consider a conical scratch device [schematic diagram in Fig. 4(a)], which is routinely used in micro- and nanoscratch applications [14]. In these tests, the protocol typically consists of linearly increasing the vertical force, FV , along the scratch path [solid line in Fig. 4(b)], resulting in an increase of both the scratch depth and groove size. In parallel, the tangential force, FT is measured [dashed line in Fig. 4(b)]. A representative top view of the resulting scratch path is presented in Fig. 4(c). 204302-3 PRL 106, 204302 (2011) PHYSICAL REVIEW LETTERS b) 100 a) (prescribed) (measured) 80 60 40 20 0 c) 0 1 2 3 4 5 0.5mm d) 200 150 900 100 600 50 300 0 0 1 2 3 4 AE (Counts ) 1200 0 5 FIG. 4 (color online). (a) Schematic diagram of the conical indenter; see text for the geometrical details of the probe. (b) Prescribed vertical and measured tangential forces during the scratch test. The vertical force FV is linearly increased and the resulting tangential force FT is recorded. (c) Photograph of the residual groove obtained after the scratch test, where the scratched region appears as light gray. (d) Fracture scaling of the microscratch test (left axis) and acoustic emission associated with the fracture process (right axis). Dashed and dotted lines represent mean value st. dev. for the conical probe region. To simplify the analysis, the vertical force is assumed to be entirely submitted through the contact area into the material. To first approximation, we assume a constant uniaxial stress xx ¼ FTR=A over the projected (load bearing) contact area A ¼ ðSÞ nx dS so that ti ¼ ij ni ¼ xx nx . Following the same procedure for the contour integral of the energy release rate, pﬃﬃﬃﬃﬃﬃﬃﬃﬃthe general form for the fracture criterion yields, FT = 2pA ¼ Kc . For a conical scratch device of half-apex angle , perimeter p ¼ 2d= cos and projected contact area A ¼ d2 tan, we obtain: sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ FT tan : (7) ¼2 cos Kc d3=2 To validate this fracture scaling, we carried out scratch tests on steel with a Rockwell diamond probe. This conical probe of half-apex angle ¼ 60 ends in a hemispherical tip with mean radius R ¼ 200 m, which transitions from the sphere to the cone at d=R ¼ 0:132 [see schematic in Fig. 4(a)]. In Fig. 4(d) we present the scaling of FT =d3=2 vs the scratch path, X, for a microscratch test on steel. In this experiments, FV is linearly imposed from zero to 100 N week ending 20 MAY 2011 [Fig. 4(b)] resulting in a variable depth up to 47 m and a residual groove along a 5 mm scratch path [Fig. 4(c)]. The most important feature that emerges from the data shown in Fig. 4(d) is that FT =d3=2 converges towards a straight line in the region of the conical probe, where acoustic emissions [15] provide strong evidence that a fracture process is indeed at play. Through Eq. (7), we determine the fracture toughness pﬃﬃﬃﬃ of the material at microscales, Kc ¼ 40 0:2 MPa m, a value that is consistent with pﬃﬃﬃﬃtypical macrotoughness values for steel, Kc ¼ 50 MPa m [16]. In summary, we have uncovered that scratching is a fracture dominated process. The model we have proposed and validated through well-controlled experiments provides a readily applicable methodology to determine fracture toughness of materials. The scalability of our approach opens new venues towards further miniaturization of this technique, to extract fracture properties of materials at even smaller length scales. We are grateful to B. Lecampion (Schlumberger) and C. Germay (Epslog Engineering) for the data on cement paste and Jurassic limestone, to N. X. Randall for making available the CSM Instruments Revetest Testing System [14], and to J. Germaine, S. Rudolph, H. Ryan and J. Miller for technical assistance. *To whom all correspondence should be addressed. [email protected] [1] D. T. Tabor, Proc. Phys. Soc. London Sect. B 67, 249 (1954); M. E. Broz, R. F. Cook, and D. L. Whitney, Am. Mineral. 91, 135 (2006). [2] H. Ollendorff and D. Schneider, Surf. Coat. Technol. 113, 86 (1999). [3] F. Wredenberg and P. L. Larsson, Wear 266, 76 (2009). [4] G. Schei et al., SPE Journal, doi:10.2118/63255-MS (2000). [5] J. G. Thacker et al., Clin. Plast. Surg. 4, 167 (1977). [6] G. I. Barenblatt, Adv. Appl. Mech. 7, 55 (1962). [7] G. P. Cherepanov, Appl. Math. Mech. 31, 503 (1967). [8] J. R. Rice, J. Appl. Mech. 35, 379 (1968). [9] The divergence theorem allows a change of the volume integral in Eq. (3) into a surface integral and we also make use of the fact that in a displacement-controlled fracture test the displacement rate seen by the moving observer is _ i;x . equal to ui;t ¼ ‘u [10] A. A. Griffith, Phil. Trans. R. Soc. A 221, 163 (1921). [11] A-T. Akono and F-J. Ulm, Eng. Fract. Mech. 78, 334 (2011). [12] B. Cotterell and Y. W. Mai, J. Mater. Sci. 22, 2734 (1987). [13] X. Wu and F. Wittman, Eng. Fract. Mech. 65, 209 (2000). [14] N. X. Randall et al., Surf. Coat. Technol. 137, 146 (2001). [15] T. R. Wilshaw and R. Rothwell, Nature (London) 229, 155 (1971). [16] W. T. Matthews, Plane Strain Fracture Toughness (KIc) Data Handbook for Metals, AMMRC MS73-6 (U. S. Army Materials and Mechanics Research Center, Watertown, MA, 1973). 204302-4

Download
# Scratching as a fracture process: from butter to steel Please share